 •Foreword
 •Foreword to First Edition
 •Contributors
 •Preface
 •A.1 Piezoelectric Materials
 •A.3 Optical Fiber Sensors
 •A.4 Electrorheological Fluids
 •A.5 Magnetostrictive Materials
 •A.6 MicroElectroMechanical Systems
 •A.7 Comparison Of Actuators
 •References
 •Index
 •1. Introduction and Overview
 •1.1 General
 •1.3 HighPerformance Fiber Composite Concepts
 •1.4 Fiber Reinforcements
 •1.5 Matrices
 •References
 •Bibliography
 •2. Basic Principles of Fiber Composite Materials
 •2.1 Introduction to Fiber Composite Systems
 •2.3 Micromechanics
 •2.4 Elastic Constants
 •2.5 Micromechanics Approach to Strength
 •2.6 Simple Estimate of Compressive Strength
 •References
 •3. Fibers for PolymerMatrix Composites
 •3.1 Overview
 •3.3 Carbon Fibers
 •3.4 Boron Fibers
 •3.5 Silicon Carbide
 •3.6 Aramid Fibers
 •3.7 Orientated Polyethylene Fibers
 •3.8 Dry Fiber Forms
 •References
 •4. Polymeric Matrix Materials
 •4.1 Introduction
 •4.2 Thermoset and Thermoplastic Polymer Matrix Materials
 •4.3 Thermosetting Resin Systems
 •4.4 Thermoplastic Systems
 •References
 •5. Component Form and Manufacture
 •5.1 Introduction
 •5.2 Outline of General Laminating Procedures
 •5.5 Filament Winding
 •5.7 Process Modelling
 •5.8 Tooling
 •References
 •6. Structural Analysis
 •6.1 Overview
 •6.2 Laminate Theory
 •6.3 Stress Concentration and Edge Effects
 •6.4 Failure Theories
 •6.7 Buckling
 •6.8 Summary
 •References
 •7. Mechanical Property Measurement
 •7.1 Introduction
 •7.2 Coupon Tests
 •7.3 Laboratory Simulation of Environmental Effects
 •7.4 Measurement of Residual Strength
 •7.5 Measurement of Interlaminar Fracture Energy
 •References
 •8. Properties of Composite Systems
 •8.1 Introduction
 •8.3 Boron Fiber Composite Systems
 •8.4 Aramid Fiber Composite Systems
 •8.6 Properties of Laminates
 •References
 •9. Joining of Composite Structures
 •9.1 Introduction
 •9.2 Comparison Between Mechanically Fastened and Adhesively Bonded Joints
 •9.3 Adhesively Bonded Joints
 •9.4 Mechanically Fastened Joints
 •References
 •10. Repair Technology
 •10.1 Introduction
 •10.2 Assessment of the Need to Repair
 •10.3 Classification of Types of Structure
 •10.4 Repair Requirements
 •10.6 Patch Repairs: General Considerations
 •10.7 Bonded Patch Repairs
 •10.9 Application Technology: In Situ Repairs
 •10.10 Bolted Repairs
 •References
 •11. Quality Assurance
 •11.1 Introduction
 •11.2 Quality Control
 •11.3 Cure Monitoring
 •References
 •12. Aircraft Applications and Design Issues
 •12.1 Overview
 •12.2 Applications of GlassFiber Composites
 •12.3 Current Applications
 •12.4 Design Considerations
 •12.7 A Value Engineering Approach to the Use of Composite Materials
 •12.8 Conclusion
 •References
 •13. Airworthiness Considerations For Airframe Structures
 •13.1 Overview
 •13.2 Certification of Airframe Structures
 •13.3 The Development of Design Allowables
 •13.4 Demonstration of Static Strength
 •13.5 Demonstration of Fatigue Strength
 •13.6 Demonstration of Damage Tolerance
 •13.7 Assessment of the Impact Damage Threat
 •References
 •14. ThreeDimensionally Reinforced Preforms and Composites
 •14.1 Introduction
 •14.2 Stitching
 •14.3 ZPinning
 •14.6 Knitting
 •14.8 Conclusion
 •References
 •15. Smart Structures
 •15.1 Introduction
 •15.2 Engineering Approaches
 •15.3 Selected Applications and Demonstrators
 •References
 •16. KnowledgeBased Engineering, ComputerAided Design, and Finite Element Analysis
 •16.2 Finite Element Modelling of Composite Structures
 •16.3 Finite Element Solution Process
 •16.4 Element Types
 •16.5 Finite Element Modelling of Composite Structures
 •16.6 Implementation
 •References
562 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES
The geometric model is also not exact. I f the finite elements are based on an assumption that the fibers remain in their design orientation and are not realigned in the draping process, then the solution will converge to the exact solution for this configuration. The analysis described above using rod elements will also give no information about the detailed stresses at the point where the tube crosssection changes. A planar axisymmetric or full threedimensional analysis, which includes the geometry detail where the section changes, is required to generate these stresses.
At the end of Step 6, the analyst has information available to help make decisions about the accuracy of the modelling process. If a linear analysis was executed, the stress levels can be checked to determine whether the value of the stiffness modulus used in Step 3 was appropriate and the displacements can be checked to determine whether the predicted deformation of the structure is sufficient to introduce nonlinear effects due to geometry change. If the answer to either question is "yes" then a nonlinear analysis is required and the analysis returns to Step 3 with appropriate algorithms to update the solution and iterate towards the correct result.
16.4Element Types
A finite element system contains a library of finite elements,6 as indicated in Figure 16.11. The most general threedimensional representation is given by brick elements. In a micromechanical model, these elements can be used to model individual fibers and resin to investigate, for example, stresses caused by thermal shrinkage of the resin relative to the fiber in the failure theories considered in Chapter 6.
For problems involving the behavior of structural components, such as the spoiler in Figure 16.3 models built with bricks can involve an unmanageable number of elements. A feature of digital computers is that the storage of numbers and performance of algebraic operations is not exact but is determined by the number of digits used to represent each number in the computer memory. If a brick element becomes long and thin, its stiffness in the shorter dimensions becomes much higher than its stiffness in the longer dimensions [see the dependence on 1//L in equation (16.1)]. Bending stiffness can vary with the cube of the length, and therefore only a moderate aspect ratio can be achieved before the terms in equation (16.3) will have vastly different magnitude and numerical instability becomes a problem.4 The rule is that brick elements should be simple cubes, or at least should be of moderate aspect ratio. Therefore, if the crosssection of a structural beam or a thin plate was to be modelled with bricks, an extraordinary number of cubelike elements would have to be used.
To overcome these problems, finite element systems include elements that are based on beam, plate, and shell theory. These theories have been developed by engineers to analyze special structural configurations. The beam element is used for structural members for which the required stiffness and load paths can be
KNOWLEDGEBASED ENGINEERING, CAD, AND FEA 
563 
represented by onedimensional straight and curved elements. The calculations in the plane of the section are completed mathematically when the element is formed. The finite element model is then used to determine the response dependent on the axial stiffness, EA; the bending stiffness, EI; and the torsional stiffness, GJ. The difference in stiffness in the plane of the section compared with the longitudinal axis of the beam is then removed from the analysis.
The same is true for plates. The plan dimensions of a brick representing a plate are limited by the throughthickness dimension. Therefore, a large number of bricks are required to model a relatively simple plate. A brick model of the assembled set of plates that comprise a structure, such as that presented in Figure 16.3, is usually not feasible. However, if the limitations defined at the beginning of Chapter 6 are acceptable, the assumption that the strain varies linearly through the thickness can be used to integrate the throughthickness behavior as the elements are assembled, leaving the deformation defined by midplane strains and curvatures.
Plate elements are therefore twodimensional and lie on the midplane of the surface they represent. The size of the elements is not linked to the thickness of the plate and the mesh requirement is that the elements be 'nearsquare' in plan view and small enough to capture the variation in stresses and strains caused by geometry features in the plane of the plate. A shell is similar to a plate, but the surface can be curved.
16.5Finite Element Modelling of Composite Structures
Structural laminates can be modelled using the twodimensional planar plate elements. Beams of various sections can also be assembled from plate elements if plate elements are used to represent the webs and flanges of the beam. In this approximation, the stresses acting through the thickness are not modelled. A pressure load applied to the plate can be approximated as varying linearly from the value equal to the applied pressure at the surface on which the pressure is applied, to zero, on the unloaded surface. Shear stresses with throughthickness components are defined in a postprocessing process that applies plate theory.
If accurate throughthickness stresses are required, the model must be based on threedimensional elements with, at least, one brick element in the throughthickness direction for each stack of plies with the same orientation.
The simplification of the model to onedimensional rod and beam elements involves significant approximations and is only implemented when the beams are slender and simple axial deformation and bending theory is a good approximation to the structural response.
The steps taken in Section 16.3 are the same whether the structure is made from metal or composite. In the derivation of all types of finite elements, the modification required to allow the analysis of composite rather than a metal structure lies only in the definition of the material propertiesthe relationship between stress and strainin Step 2.
564COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES
16.5.1Plate and Shell Elements
Plate and shell elements can be used to model structures composed of laminates such as the wing spoiler in Figure 16.3.
16.5.1.1 Plate and Shell Elements for Laminates Constructed from
Orthotropic Ply Material For laminates constructed from orthotropic plies, the laminate theory of Chapter 6 is used to define the properties of the plate elements. Preprocessors in finite element systems allow the layup to be defined. First, a set of orthotropic properties is defined for the unidirectional or fabric plies to be used in the laminate. A tabular input is then used to define the orientation, thickness, and material for each ply. The properties required for the plate are then automatically calculated. As an added feature, the coefficients Aij, Bij, and Dij defined in the laminate theory can be listed together with the effective orthotropic elastic constants E11, E22, etc.
16.5. 1.2 Woven and Knitted Material (Unit Cell Approach). Defining the elastic constants for a woven material is more complex, and a unit cell approach is often adopted. 7 In this approach, equivalent elastic constants are derived using a detailed finite element model of a representative unit cell. Actual fiber architectures are modelled using brick elements for the fiber tow and resin. Displacements are then applied to the cells to isolate the effective longitudinal, bending, and torsional components of deformation required to define the elastic matrices describing the laminate behavior. These constants are then available for subsequent analyses.
16.5.1.3 Brick Elements. Brick elements can be used to model individual layers in a laminate, or a single element can be used to model several layers. When used to model layers, an "average" property for the combination of resin and fibers has to be defined. The stressstrain relationship for a general anisotropic material involves all 21 coefficients in the symmetric matrix [G] defined below. The 21 coefficients are defined in terms of 12 elastic constants.
The threedimensional stresstostrain relationship for an orthotropic material representing a layer of fabric or unidirectional tape is simpler and is defined by:
O'y 
Sy 

~y 
o~ = [6"1 
8z 
 ( r  r R e v ) 
~z 
or4 

r ~ 
y~y 


•z 
Yyz 

as 
rzx 
Yu 
a6 
Тут вы можете оставить комментарий к выбранному абзацу или сообщить об ошибке.
Оставленные комментарии видны всем.